|Monthly Tech-Tip |
The logo on the left was rubber-stamped using and ink mix made of only glycerine and Mason 6666 black stain. The glaze is shedding off during firing. Multiple properties needed by a stamping ink are not present here. First, the stain dries as a powder, it has no hardening or bonding properties, glycerine is its only mechanism. Second, it is too concentrated, the black color is so powerful that it bleeds excessively into the overlying glaze. Third, it does not melt during firing so it does not bond with the body below. And, it either develops only a fragile interface with the glaze above, or sheds it off. The piece on the right mixes the stain 50:50 with a glossy transparent glaze (having 20% kaolin), it lays down better, accepts the overglaze layer better (because it has less glycerine), presents less problems in handling before glazing and it has no issues with the overglaze crawling off during firing. Black stains are potent, a 75:25 stain:glaze mix would work even better.
Blend the two types, permanent and washable, with a powdered colorant, in the proportions appropriate to get as much hardness as possible but not so much that it is difficult to clean up the screen. The powder should be a ceramic stain mix with a melter medium (a glaze or frit).
On the left is a pure blue stain, on the right a green one. Obviously, the green is much more refractory. On the other hand, the green just sits on the surface as a dry, unmelted layer. For this type of work, stains need to be mixed into a glaze-like recipe of compatible chemistry (a medium) to create a good, paintable color. The blue is powerful, it would only need to comprise 5-10% of the recipe total. Its medium would need to have a stiffer melt (so the cobalt fluxes it to the desired degree of melt fluidity). A higher percentage of the green stain is needed, perhaps double. It's medium needs much more melt fluidity since the stain is refractory. Of course, only repeated testing would get them just right. Guidelines of the stain manufacturer for chemistry compatibility need to be consulted also (as certain stains will not develop their color unless their glaze medium host has a compatible chemistry). And, to be as paintable as possible, use use a gum-solution/water mix (e.g. 2 parts water to one part gum solution).
It is a mistake to use pure stains for decorating ware. Stains need to be mixed with a ceramic carrier and a working medium to work and fire well.
Silk screen printing
Silk screen printing is one of the best options for hobbyists and potters to reproduce crisp and detailed decoration. But there are many details to know.